POLITECNICO DI TORINO
Collegio di Ingegneria Energetica
Corso di Laurea Magistrale
in Ingegneria Energetica e nucleare
Tesi di Laurea Magistrale
EXPERIMENTAL INVESTIGATION OF THERMAL STORAGE USING WASTE MATERIAL
prof. Papurello Davide
Candidato Tommaso Pavone
The study, which will be described in the following chapters, focuses on the energy feasibility of organic waste materials for their possible application in thermal storage systems as phase change material.
First, we have briefly described the generality of possible energy storage solutions, focusing mainly on the thermal storage systems. Thermal energy storage (TES), with various types of phase change materials, were investigated considering the exploitation of their latent heat.
Among the commercial materials, it was chosen a paraffin wax, while as innovative materials were chosen fatty materials of animal origin. This is a circular material approach in order to reuse also such kind of wastes from kitchens and restaurants refuses. The products chosen for the analysis are lard, butter and animal fat obtained from a previous cooking phase. This last material has been chosen in such a way that, unlike the others, it is possible to determine if an organic waste can be an optimal solution for the thermal storage in order to lower the investment costs for the storage thermal system.
Furthermore, it was decided to carry out the same procedures with paraffin, which, in the phase- change thermal accumulations, is the most used material for these types of systems.
A first phase of laboratory tests was carried out. This makes possible to check whether the chosen materials are able to reach the temperatures typical of a TES system and if at those values, the materials chosen reach the melting temperature for the latent heat storage.
A second test phase consists in the scaling simulation of a TES system. It consists in the introduction of a further layer of the phase change material to simulate a possible accumulation phase.
Experiments were carried out in laboratory, with a specific test rig and, in parallel such experiments were simulated using COMSOL Multiphysics 4.3a software.
These simulations have been made in such a way as to be able to reproduce a more ideal situation of the built systems and to check how far they differ from the analyzes carried out in the laboratory.
Furthermore, with the help of the Applied Science and Technology Department (DISAT), materials were analysed using the DSC (Differential Scanning Calorimetry) study. This analysis was used to calculate the latent heat storage, the temperature of melting and solidification. Subsequently, these data were used for the evaluation of the specific heat at constant pressure that the material assumes during the charging and discharging phase.
IV This has served to verify and to quantify such materials at the operating temperature of a typical domestic hot water request (DHW). This energy would be useful to understand if the materials considered can be excellent substitutes in the thermal storage systems to the phase change materials generally used.
1. INTRODUCTION... 1
1.1 STORAGE SYSTEMS ... 2
1.2 TYPES OF STORAGE SYSTEMS ... 3
1.3 THERMAL STORAGE ... 7
1.3.1 SENSIBLE THERMAL STORAGE ... 8
1.3.2 LATENT THERMAL STORAGE ... 10
2. LATENT HEAT STORAGES... 12
2.1 TYPOLOGY OF MATERIAL ... 12
2.1.1 INORGANIC MATERIALS ... 13
2.1.2 ORGANIC MATERIALS ... 15
2.1.3 EUTECTIC MATERIALS ... 17
2.1.4 NON-EUTECTIC MATERIALS ... 18
2.2 TYPES OF APPLICATION ... 19
3. ORGANIC PHASE CHANGE MATERIAL... 22
3.1 ORGANIC PARAFFINIC MATERIALS ... 23
3.2 NON-PARAFFINIC ORGANIC MATERIALS ... 26
3.3 NON-PARAFFINIC ORGANIC MATERIALS EXAMINATED ... 29
3.3.1 LARD ... 29
3.3.2 BUTTER... 30
3.3.3 MEAT FAT ... 35
3.3.4 PARAFFIN WAX ... 36
3.4 DSC ANALYSIS ... 37
4. EXPERIMENTAL PHASE... 43
4.1 TESTS ON SMALL SYSTEM... 44
4.1.1 MATERIAL UESD ... 44
4.1.2 ASSEMBLY PHASE ... 45
4.1.3 SIMULATION WITH COMSOL MULTIPHYSICS SOFTWARE ... 51
4.2 EXPERIMENTATION IN SCALE ... 59
4.2.1 MATERIAL USED ... 59
4.2.2 ASSEMBLY PHASE ... 60
4.2.3 SIMULATION THROUGH COMSOL MULTIPHYSICS SOFTWARE ... 66
5. RESULTS... 71
5.1 SMALL THERMAL STORAGE ... 72
5.1.1 LARD ... 72
5.1.2 BUTTER... 79
5.1.3 PARAFFIN WAX ... 85
5.1.4 FAT... 92
5.2 SCALE REPRODUCTION ... 99
5.2.1 LARD ... 99
5.2.2 BUTTER... 105
5.2.3 PARAFFIN EAX... 110
5.2.4 FAT... 116
5.2.5 AIR ... 121
5.3 RESULTS OF THE DSC ANALYSIS ... 125
5.3.1 LARD ... 126
5.3.2 BUTTER... 128
5.3.3 PARAFFIN WAX ... 129
5.3.4 ANIMAL FAT... 131
6. CONCLUSIONS... 133
The uncontrolled use of fossil fuels in industrial production processes has led to a substantial increase in greenhouse gases (GHG) of CO2 and CO into the atmosphere.
These emitted gases create extensive natural damage, primarily global warming, as greenhouse gases, triatomic and diatomic molecules create the phenomenon of absorption and scattering of solar rays.
The first one would correspond to the absorption of solar rays by the triatomic molecules and the greenhouse gases. This will avoid that the sun's rays, reflected from the earth's surface, are released into space. The scattering phenomenon would correspond to the reflection, by the diatomic molecules, of the reflected solar rays coming from the Earth's surface.
These phenomena, therefore, have caused, especially in recent years, an increase of temperatures that have caused damage to the Arctic ice cap with a reduction in its extension.
This will cause the rise of sea levels and the deep damages of crops due to the uncontrolled weather changes.
Through previous studies, it has been established that, since 1751, the various industrial chains have issued approximately 347 billion tons of gas. That is why, especially in recent years, we are trying to study and to apply alternative energy processes that are especially low emissions of harmful gases. It is mainly talking about renewable energy sources from which they are obtained from natural sources present in nature: solar, geothermal, hydroelectric and wind energy.
Among the sources mentioned above, the most interesting is the solar source. The International Energy Agency (IEA) estimated that in 2050, 21% of the world's electricity produced will come from solar sources.
In the last 3 years, the production of energy produced from solar sources has increased by 35%
and, despite still having a very low share compared to the remaining renewable sources. 
While in 2050, 16% of the thermal energy used for heating and cooling of buildings will be covered by solar thermal systems.
However, the use of solar systems, both thermal and photovoltaic, finds problems of various kinds: the intensity of solar radiation varies with the geological position, daily and the seasonal period, but above all depends on local weather conditions. In fact, a negative factor in the energy systems that use the solar source is the fluctuating variation in the hours of light and darkness.
2 This problem is relevant, above all for this technology, precisely because the highest peaks in the demand for thermal and electrical energy are mainly in the dark hours where it is not possible to make full use of renewable sources with solar energy.
This fluctuation of thermal and electrical energy demands is found in high energy production applications from renewable sources.
The accumulation function has been introduced to deal with this disadvantage and reduce the gap between production and demand of energy.
In fact, the primary purpose of placing the storage system in the energy production system is to increase efficiency.
The accumulation system has been more incentivized, in the last few years since we have obtained excellent results, also from the economic point of view.
1.1 STORAGE SYSTEMS
As already mentioned above, one of the main disadvantages of renewable energy source systems is the variability and the difficulty of matching between the energy demand and its production. In fact, the phases of greater energy demand, mainly thermal and electrical, occur in periods when there are low quantities of energy producibility; just as there are daily periods in which the opposite effect occurs.
A huge waste of energy occurs. This is caused by the amount of unused energy that is dispersed in the environment.
It is for this reason that storage systems are believed to play a key role in the renewable energy production plant, to obtain greater availability and economic advantage of intermittent sources in order to meet the energy demand.
Benefits that will be obtained adopting an accumulation system for a RES plant are:
- Reduction of energy costs;
- Reduction of energy consumption;
- Greater operating flexibility;
- Reduction of initial investment and maintenance costs;
- Reduction of dimensions of production plants;
- Increased energy efficiency;
- Reduction of the environmental impact of energy generation systems.
3 1.2 TYPES OF STORAGE SYSTEMS
A generic energy process is mainly subjected to losses and through certain energy storage techniques is possible to compensate for the low flexibility of fuels for the benefit of others.
The thermal storage is one of the most used energy storage system. A portion of thermal energy that can be lost is reused for a secondary purpose.
For each type of application we tried to apply the most appropriate storage system solution:
a) Mechanical and hydraulic systems
One of the first mechanical energy storage application system is the flywheel whose main purpose is to limit the excesses of mechanical energy on total mechanical work in periodic machines.
The flywheel is mainly opposed to any variation in its angular velocity, trying to obtain a stability of the rotation of the driving shaft when a periodic driving torque is applied.
Figure 1Typical flywheel 
Moreover, it is exploited for the accumulation of mechanical energy produced by an engine that delivers low power for a long period, and then releases it to higher powers in shorter periods.
With regard to this the flywheel has as its fundamental principle, that of accumulating the mechanical energy produced by the rotation of the tree in kinetic energy. This particular conversion was then exploited in other application fields, such as reversible electric machines in the field of propulsion and transport.
While for the hydraulics sector, one of the most intuitive systems for accumulation is the pumping system.
4 The pumping system consists in pumping water from the valley upstream at night when the energy demand is lower and the electricity costs are lower, and sent downstream during the day when there are greater peaks of electricity.
Figure 2 Pumping process during the day
Figure 3 Pumping process during the night 
b) Compressed air storage
This type of application is used in periods of low electricity demand and therefore exploiting the excess energy produced by the plant. In the post-compression phase, the air is stored in an underground cavity and then withdrawn in periods of greater energy demand.
5 So during the night, when the cost of electricity is low, we try to compress as much air as possible to generate electricity, taken from the grid, during the compression phase.
During the night the cost of electricity is higher, and then the compressor must work for short period. In this case, the compressor is the component that needs the greatest amount of energy taken from the electricity grid.
So compressed air is stored in the underground quarry at an almost constant pressure of around 70 bar.
During periods of peak demand, the air is released and heated with natural gas or with compressed air coming from the compressor, and then it is expanded inside the turbines.
Figure 4 Typical CAES system 
c) Electrochemical batteries
This type of accumulation system is the most common and readily available solution. It accumulates energy in the form of chemical energy and releases it as electricity.
6 Batteries are equipped with high stability energy and power density. The most common type of battery is the Pb/acid.
They are used in many types of applications, including heat load management, electric vehicles and renewable energy storage.
They can easily replace the pumping or compressed air systems when the demand capacity is limited.
This accumulation system has a good efficiency that is between 70-80%.
d) Magnetic storage
Energy can also be stored in the form of magnetic energy, created by the passage of current inside a coil, consisting of a semi-conductive material, subjected to cryogenic techniques.
To increase the amount of energy that can be stored and the speed of energy storage, the same procedure can be carried out using high-performing superconducting materials.
These materials are characterized by an electrical resistance considered negligible which determines a leak-free current flow. However, these losses will be considered when a current from alternating current is carried out and a loss of 10-20% occurs.
e) Hydrogen production as storage tool
Hydrogen is not first considered as a source but as an energetic vector, since there is no need for a preliminary phase of production of the gaseous material since there is no pure in nature.
Hydrogen is considered as a very interesting energy carrier because it is possible to store it and transport it very easily.
The negative factor to consider for this material is the fact that the costs of electricity, on which we must go to save during periods of peak demand, are lower than the cost of the electricity itself exploited for the production of hydrogen itself.
One of the major difficulties in the use of this gaseous material as an energy carrier is the accumulation phase itself, since to accumulate it requires a large amount of storage space and high-performance materials that can contain the hydrogen within the control volume.
It is for this reason that to make the storage phase less problematic it is possible to liquefy the gaseous material to make the fluid more inert and the possibility of leakage and breakage of the containment material being less risky.
7 f) Thermal storage
The thermal storage phase is one of the most used and easiest to reproduce systems among the various storage systems mentioned above. This storage technology determines the possibility of storing large quantities of thermal energy and then reusing them in successive phases.
The thermal energy can be accumulated in various forms but in this case we tried to carry out a more detailed study in the following chapters.
1.3 THERMAL STORAGE
Thermal storage systems can be grouped into two types depending on the type of material used as energy vector for the thermal storage phase.
The accumulation system that causes the variation to increase the temperature of the material is called sensible storage; while the accumulation of heat that causes the phase change of the material is called latent storage.
Principally, the storage system is designed to operate cyclically by applying a classification on the type of storage duration.
- Short term accumulation: exploited mainly to cope with peaks in heat energy requests of a few hours per day. This system is mainly used to reduce the size of the energy production plants but above all to take advantage of the cheaper hourly rates.
- Medium or long term accumulation: mainly used to conserve heat over longer periods of time ranging from a few weeks to months.
The long-term ones, above all, take advantage of seasonal climate changes.
These types of accumulation for medium and long-term purposes have efficiencies that are around 70% compared to 90% of short-term systems.
Another possible classification mode is based on the operating temperature. The reference temperature of these storage systems is 120 ° C. In fact, if the operating and storage temperature has a temperature lower than 120 ° C these accumulations are part of the low temperature accumulations. These systems mentioned above are interesting because the losses are more contained and therefore require lower thermal powers.
As mentioned previously, thermal storage systems are widely used and are basically designed to operate cyclically and would therefore entail beneficial purposes when they achieve the following purposes.
8 - Increase generation capacity, which would consist in the application of an energy production unit that its main objective is not to cover the peaks of energy demand but to work at higher power loads;
- Increase in the operation of cogeneration plants, which would therefore allow the cogeneration system to free itself from the demands of the load curve;
- Purchase of electricity at the most economically convenient times;
- Improved reliability of production systems;
- Integration with other energy alternatives.
1.3.1 SENSIBLE THERMAL STORAGE
For the first type of storage system, the amount of thermal energy is commonly stored in the water.
It is used for its modest costs, for its easy availability, for its high specific heat, for the easy transport and for the short transmission duration of heat.
The design phase of the storage tanks is fundamental. In fact the purpose is to create tanks that are able to maintain optimal thermal stratification and thermal insulation from the outside.
The generic thermal storage process can be composed of three steps:
- Charge phase;
- Storage phase;
- Discharge phase.
Figure 5 The three phases of a typical storage
9 Thus, in summary, the main purposes of the storage tanks for sensible storage are:
- Guarantee of thermal stratification, which consists in a clear diversification and separation between zones at different temperatures. In fact, it is essential to try to avoid mixing the zones at different temperatures as it would cause an increase in the probability of thermal dispersions towards the outside;
Figure 6 Stratification into sensible thermal storage
- Minimization of dead zones;
Figure 7 Dead zones in thermal storages
- Minimization of losses and infiltrations of heat towards outside.
10 1.3.2 LATENT THERMAL STORAGE
Latent thermal storage systems represent the most interesting alternative to the sensitive heat storage system. In general, it consists of a material that exploits the amount of heat used to chance its phase of material (PCM).
Figure 8 Difference between sensible (a) and latent(b) heat storages 
Therefore the material, used for this type of application, is a phase change material in which the temperature remains constant during the storage period, and therefore at the second step of the cycle.
From the figure 8, it is possible to notice how the latent heat storage system mainly exploits the central phase, in which the phase change material develops and where the temperature remains constant.
The latest studies consider and treat the advantageous properties of PCMs that would allow a wide possibility of application in order to have a better alternative to other types of storage systems.
Unlike any material used for a sensible heat storage system, the phase change is characterized by a high latent heat and specific heat that would allow it to accumulate as much heat energy as possible.
One of the major disadvantages of PCM is their low conductivity which makes the process slower and therefore one of the main purposes is to increase the speed of heat transmission in the medium to make the charge and discharge phases faster.
11 So in the subsequent studies we will make a study more in depth those characteristics that will be increased in order to improve the various phases.
Unlike a sensible heat storage system, where one of the main purposes is to maintain a thermal stratification along the entire control volume, the latent heat can be decomposed into several zones at different melting temperatures, so as to satisfy more loads at different temperatures.
Figure 9 Difference between stratification of sensible heat storage and temperature zones od PCMs 
For a good sizing of a latent heat storage system with phase change material it is recommended to take into consideration the following characteristics:
- Range of temperature of the storage system and the fluid flow rate for the thermal exchange;
- The type and characteristics of PCM;
- Matching between the amount of energy accumulated and released by the system;
- Comfort requirement.
In summary, it is possible to determine the elements that characterize the choice of a PCM: a) Thermo-physical properties:
- Easiness of choice of material based on the operating temperature range;
- High conductivity good heat transmission properties;
- High latent melting heat per unit of mass;
- Thermal stability;
- Phase stability and no segregation;
12 - Low volume for the charging phase;
- Low saturation pressure at operating temperature;
b) Kinetic properties:
- High degree of nucleation and no undercooling in the liquid phase;
- High degree of crystallization;
c) Chemical properties:
- Complete fusion and solidification cycling;
- Long-term stability and lack of degradation after several melting and solidification cycles;
- Chemical stability;
- No toxicity, flammability and explosiveness;
d) Economic properties:
- Abundance and availability;
- Low economic value;
e) Environmental properties:
- Low energy incorporated;
- Easy separation from other materials and recycling potential;
- Low environmental impact and low pollution.
2. LATENT HEAT STORAGES
As already well defined above, the storage system is mainly used by renewable energy plants.
Phase change materials must have specific properties including the melting and solidification temperature that must be in accordance with the type of application on which to install the storage system.
2.1 TYPOLOGY OF MATERIAL
Considering several literature studies carried out, it was determined a precise classification of phase change materials used.
The PCMs of interest are divided into:
13 - Inorganic;
- Not Eutectics.
2.1.1 INORGANIC MATERIALS
As shown in the above graph, the main inorganic PCMs are subdivided into hydrated salts and metals.
Regarding the first category, hydrated salts are one of the most used as phase-change accumulation material among inorganic ones.
Figure 10 Hydrated salts (a), metals (b)
14 Regarding this material, this can be considered as a material that works at medium-low temperatures, and therefore they are highly exploited precisely because they can be applied to a large quantity of energy applications.
Like any phase change accumulation material, in contact with a hot fluid it takes heat and then releases it with a cold fluid and with this last process the material is characterized by the crystallization of the body.
One of the most important disadvantages of hydrated salts is the under-cooling which is mainly due to the speed at which the heat release phase occurs.
Another inorganic material belonging to this category are the molten salts which are characterized by a low thermal conductivity and that is why the accumulation component is optimized by mixing them with materials, of metallic nature, or the duct, in which the fluid passes, is integrated with a finning to increase the heat exchange surface.
The other category belonging to phase change accumulation materials are metals that, unlike previous materials, have a high thermal conductivity and a high latent heat.
Having these particular properties the material works at much higher operating temperatures and having excellent thermal conductivity, the probability of dispersion of heat towards the outside of the control volume is much higher, and therefore to avoid this inconvenience the volume containment material is integrated with a thick layer of insulation to contain losses.
Based on the studies carried out, it was possible, especially for hydrated salts, to identify the advantages of using the material in a storage system:
- High heat of volumetric accumulation and high melting enthalpy;
- High melting heat;
- Quick exchange phase;
- High thermal conductivity;
- Possibility of using small exchange volumes;
- Compatibility with plastic materials;
- The use of hydrated salts is preferred to organic materials as paraffin to obtain a better reduction of environmental impact in the manufacturing phase;
In addition, always through the studies carried out on the hydrated salts, as well as the other inorganic accumulation materials, we have highlighted the disadvantages that would make the accumulation process less efficient:
- Low nucleation properties and under-cooling problems;
15 - Inconsistencies in the temperature of function during the various charging and
- During the transition phase, problems of segregation and thermal instability occur;
- Increase, during their repeated exploitation, of degradation;
- Incompatibility with some materials used for building construction, because if we install the inorganic PCM with some building components, it would make the opaque envelope of the building more unstable;
- Corrosive with some metallic and slightly toxic materials.
2.1.2 ORGANIC MATERIALS
The organic materials, as regards the thermal storage system, becomes one of the most interesting components to be exploited.
As shown in the graph above, organic materials, to be used for thermal storage systems, are subdivided into two categories, paraffinic and non-paraffinic.
The first category are mainly hydrocarbons and are characterized by a good storage capacity.
As for the category of not paraffinic storage materials, they are mainly fatty acids or, as we will see later, organic waste characterized by a good latent heat of fusion, an adequate operating temperature that can be used by many types of systems of energy production, especially from renewable sources.
Figure 11 Natural paraffin (on the left), encapsulated paraffin (on the right)
16 Through the studies carried out, to see its feasibility in the energy field, it was possible, as determined for inorganic materials, to identify positive factors in organic materials:
- Wide availability in a wide temperature range;
- High latent melting heat;
- Heat transfer and cooling of the material even for a small amount of energy and no possibility of under-cooling effects in the discharge phase;
- Phases of congruent phase changes;
- Good self-nucleating properties;
- No possibility of nucleation in phase change and good degree of nucleation.
Just as there are advantages, some disadvantages characterize the organic materials that must be tackled in such a way as to reduce negative effects and improve performance:
- Low thermal conductivity of fusion;
- Low latent volumetric heat capacity and low enthalpy quantity in the phase change period;
- Low volumetric density;
Some materials are flammable because some organic materials, especially paraffinic, are mainly hydrocarbons;
- High cost especially for paraffinic materials as their availability is low;
- High volumes, compared to inorganic materials, so that the heat exchange and accumulation phase is successful.
The organic materials used in thermal storage systems will be seen in more detail in the following chapter, as our study is based on the feasibility of using organic waste materials for thermal storage systems.
Figure 12 PMCs with their Melting temperature and Heat of fusion
17 As shown by the graph in the figure 12, while working at the same temperatures, the organic and inorganic materials have very different fusion enthalpies and as a function of this sharp difference, it is possible to apply different materials to the same energy systems.
Also from the previous graph, it is possible to notice one of the main differences between the organic and inorganic accumulation materials, that is, how the organic materials have a latent heat of fusion much lower than the inorganic ones.
2.1.3 EUTECTIC MATERIALS
The eutectic materials consist mainly of the mixture of two or more components where they are characterized by the same melting point.
These materials are practically used because a single material could have deficits that would make the accumulation phase poorly performing, and therefore mixing them with other materials with excellent energetic characteristics would make the whole component better and the whole process of energy storage more efficient.
Figure 13 Typical eutectic mixture
As can be seen from the graph, it is convenient to make the mixture work near the eutectic point, where the same melting temperature is obtained and where it is possible to take advantage of the energetic characteristics of both the materials that make up the mixture.
Unfortunately, this component, compared to the previous two, is still under study because it is a difficult task to find a good compromise between two materials that have excellent energy performance.
18 However, due to the simple fact that in order for the two mixed materials to operate at the same time they have limited use, that is, some energy systems that work at different temperatures from the melting point of the eutectic material cannot take advantage of the material itself.
2.1.4 NON-EUTECTIC MATERIAL
As for this last category, it is mainly exploited in cooling energy thermal systems. In fact, the non-eutectic thermal accumulation materials are characterized by the mixture of different materials such as to give the whole heterogeneous component with different melting temperatures.
Based on the energy point of operation of the system that exploits the material, a well-defined melting temperature, which would consist of a melting temperature of one component of the mixture or another, will be taken into account.
Having different problems regarding the exploitation of the whole material, we try to use it at low temperatures in order to take advantage of the greatest number of beneficial factors of the mixture. And this is why non-eutectic material is mainly used in cooling systems.
The use of the component only for this type of energy systems, would make its goal much more limited and therefore could not be exploited by other energy systems at higher temperatures.
Moreover, its heterogeneity would make it more difficult to exploit both components of the mixture to the maximum and that is why the non-eutectic material is used at lower temperatures.
Therefore, in conclusion, the component on which we are going to focus are non-paraffinic organic materials in such a way as to be able to verify if waste materials with energetic characteristics consistent with those of generic organic materials can have their use in the field of energy storage.
2.2 TYPES OF APPLICATION
Through the studies carried out, phase change materials can be used for a wide range of applications that mainly determine the possibility of being able to reduce energy production costs in economically unfavourable daily periods.
19 Phase change material is most often used to replace the simple materials used for energy storage for solar thermal systems.
These types of systems work mainly during the day trying to accumulate thermal energy in these hours, where the energy demand is lower, and then release it at night where the demand peaks are greater.
A limiting factor of the solar thermal plant is its intermittency and cyclicity which is disadvantageous for the thermal energy production phase. And this is why we tried to couple an accumulation system to the energy production system. An application that has been tried to develop in recent years is the possibility of being able to replace the typical storage systems with sensitive materials and with PCM, in order to reduce the costs of materials but above all space.
Figure 14 Typical latent heat thermal storage coupled with solar thermal system
There are many factors to be considered for this application in such a way that the functioning of the thermal storage system, with phase change material, is effective is the melting temperature of the PCM. In fact, the melting temperature must be at least 5 °C lower than the temperatures reached by the solar thermal system, so that the entire material is melted and the greatest possible amount of thermal energy is captured. 
It has been ascertained that, with the introduction of a thermal accumulator based on phase change material, as well as with sensitive materials, the efficiency of the solar thermal system, the solar fraction would be increased and the cost of the whole system of production (solar
20 collectors), but above all it would be possible to use the entire energy stored in dark periods where the demand for thermal energy is higher. However, through the use of the phase change materials, would also face a possibility of being able to reduce the spaces and, through the easy availability of the material, would reduce the costs of the accumulation material.
Another application on it is possible to apply PCM is the introduction of these phase change materials in the stratification of the opaque envelope of a building.
This installation aims to shift the thermal load peaks to which the building is subjected.
Figure 15 Thermal loads in a simple apartment 
In fact, both from the inside, with anthropic activities and electronic equipment, and from the outside, with weather stress, the entire opaque shell must have the possibility of being able to accumulate heat and then release it in daily periods when temperatures are more low, thus maintaining the highest internal temperature, thus reducing the use of the air handling unit and thereby reducing electricity costs.
The main purpose is to increase the thermal accumulation inside the opaque casing and to do this, various options have been made regarding the positioning of the phase change material within the stratification of the wall.
Figure 16 Different application of PCM into the stratification 
Depending on the positioning, shown in the figure 16 above from layer 3, it is possible to favour the interior or exterior of the building. If the PCM is exposed to the inside and the insulating material more towards the outside would favour the inside of the building, thus releasing the heat, produced above all by the anthropic activities, at night.
Behzadi and Farid  carried out a comparative study between a building with PCM and one without and it was concluded that the daily fluctuation is reduced by 4 °C on summer days and highlighting a significant energy saving for the air conditioning system of 34.5% and 21% in the heating of winter days.
Finally, this possibility of introducing the phase change material inside the opaque casing has opened up numerous applications such as the PCM encapsulation inside the wall itself, or how to apply the PCM on the floor using the inlets or even in the pavement.
Figure 17 Macro PCM on the wall  and on the roof 
A last application that aroused much interest is to be able to replace the air treatment unit consisting of heat exchangers, in which cold or hot water passes depending on the season, time of day and internal loads, with the PCM thus applying a free cooling system. 
Figure 18 Free cooling process 
During the night the cold air is stored by the PCM through natural ventilation and then released into the living areas during the hours of light and heat, thus obtaining results with regard to energy saving. 
Through other studies carried out, it has been noticed that the thickness of the PCM inside the ventilation system plays an important role for the heat exchange, as well as the mass flow rate of the air passing through the PCM banks.
Finally, through the application study of various types of phase change materials within the ventilation system, it was stated that the energy saving of electricity compared to the traditional ventilation systems is about 73%. 
3. ORGANIC PHASE CHANGE MATERIAL
As already mentioned in the previous paragraphs, there are four macro categories of phase change accumulation materials. Among these, those that still present a scientific interest are organic materials.
Phase change organic materials are mainly divided into two: paraffinic and non-paraffinic.
Both categories of organic materials have lower thermal properties than other accumulation components. Just think, for example, that the latent heat of fusion of inorganic materials is higher than the organic ones if they are operated at the same operating temperatures.
However, their high availability in nature and their low cost make organic phase change materials a subject of study.
23 From the first comparative studies, it has been verified that most of the phase change organic materials are excellent to be exploited by energy systems that work at different operating temperatures.
Unlike inorganic materials, or other categories, organic ones have a high instability if they are made to work at high temperatures because of the bonds that make up the material that are of covalent type.
3.1 ORGANIC PARAFFINIC MATERIALS
Paraffin waxes are the most used among phase change organic materials. It belongs to the family of hydrocarbons, mainly alkanes, characterized by chains with more than 20 carbon atoms. They are characterized by large phase change properties and have excellent chemical stability in contact with other different materials. To avoid further dispersion during phase change, it is necessary to enclose the paraffin with high thermal conductivity materials. This encapsulation, however, if it were installed inside the opaque envelope of a building, would make the entire wall much weaker if subjected to mechanical stress. 
Figure 19 Enthalpy of fusion variation belong to temperature of application 
24 As can be seen from the graph in figure 19, the paraffin have a very wide operating temperature range, comparable to that of the hydrated salts. However, what is observed is also the amount of fusion enthalpy, which has much lower values than other phase change materials.
In addition there are various types of paraffin, and this is due to the amount of carbon atoms inside the chain.
Figure 20 Various types of paraffin 
As can be seen from the previous table in figure 20, the variation in the amount of carbon atoms, it is possible to obtain a large quantity of paraffin waxes with different melting temperatures and latent heat. In fact, as the numbers of carbon atoms increase, the melting temperature increases. While the variation of latent heat of fusion depends on the amount of carbon atoms within the chain, but does not depend on their increase.
As mentioned previously, the paraffin has a temperature range, which is around 20 to 70 °C, which would then allow it to be used for a wide range of energy applications. However, paraffin, unfortunately, has a very low conductivity of about 0.2 𝑊
𝑚𝐾, thus making the phase-change accumulation phase, for each energy application, less performing.
This unfavourable condition would result in a reduction in the amount of heat transmitted in the medium and would increase the melting time of the material.
Numerous studies have been carried out in such a way as to increase thermal conductivity. A first test carried out was that of the paraffin encapsulation with a high conductivity material, as already mentioned above, or installing the organic material inside a matrix made of a material
25 with high thermal conductivity or installing a wing around the tube in which the fluid passes, so as to increase the heat exchange surface.
Finally, a very interesting study carried out by Whiffen and Riffat  would consist in mixing the paraffin with a metallic powder. In this case, the material used expanded graphite (EG).
Figure 21 Temperature variation between generic paraffin and paraffin mixed with EG 
The test was carried out because a considerable difference in level was determined from the standpoint of duration between the charge and discharge phase. In fact, the charging phase had a longer life than the solidification process of the phase change material.
As can be seen from the graph, the mixture of paraffin and expanded graphite powder allowed to reduce the time during the charging phase. This observation was determined by the simple fact that the mixture reaches the melting temperature in a shorter time than the duration of the simple paraffin wax charge phase.
The test determined that having a good percentage of mixed metal powder inside the paraffin would increase the thermal conductivity, low thermal dispersions would be obtained, chemical stability, excellent compatibility and would keep the density of the material low.
In fact, the other characteristics that make the paraffin unique, as we will see for the other organic materials, is that in addition to having good thermal qualities, and its flammability, its non toxicity and even the failure to achieve the undercooling, which we obtain in the phase of discharge and crystallization of an inorganic phase change material.
26 From what has been found, therefore, is that paraffin is an excellent competitor in the field of phase change materials.
Despite having rather low thermal characteristics, compared to other materials, modest costs, which are between 0.5 and 10 €
𝑘𝑔, paraffin waxes can be found as a phase change in thermal storage systems obtaining excellent results. 
3.2 NON-PARAFFINIC ORGANIC MATERIALS
Non-paraffinic organic materials are a very interesting alternative to generic paraffin waxes.
These components are more available than generic organic materials.
Among the non-paraffinic organic materials, most of the studies have been carried out on fatty acids.
Fatty acids are mainly composed of a long chain of carbon atoms and can be divided into two categories: saturated fats and unsaturated fats.
Figure 22 Chemical difference between saturated and unsaturated fatty acids 
As can be seen from the figure 22, the characteristic that differentiates saturated and unsaturated fatty acids is the link between the carbon atoms within the chain. In fact, in saturated fatty acids, the carbon atoms are connected to each other by single bonds while the unsaturated ones have double bonds inside their structure.
27 This sharp distinction also makes numerous types of fatty acids differentiated mainly by the melting temperature.
Formula Common Name
Formula Common Name
Melting Point CH3(CH2)10
Oleic acid 13 °C
69°C CH3CH2CH=CHCH2C H=CHCH2CH=CH(CH
From the previous table  it is possible to notice that in saturated fatty acids the melting temperature increases as the CH2 group increases, while the unsaturated fatty acids are mainly exploited in the applications that work at cryogenic temperatures.
Fatty acids are very important because they have higher thermodynamic properties than other PCMs such as fusion congruence, good chemical stability, non-toxicity that allow their use for a large number of passive solar heating applications. 
These materials, in their liquid phase, have a surface tension of the order 2-3 · 10-4 𝑁
𝑐𝑚 which is high enough to be retained in the structure of the host material.
As can be seen from the table in figure 23, the increase not only affects temperatures, but also other thermodynamic characteristics. In fact, the increase in the quantity of carbon atoms belonging to the main chain of the compound is directly proportional to the increase in melting temperature but inversely proportional to the amount of latent heat of fusion.
28 While, as regards the specific heat at constant pressure, its increase does not depend fundamentally on the number of carbon atoms of fatty acid, but its increase depends on the state of aggregation of the molecules.
Figure 23 Thermal properties for different fatty acids 
In fact, the specific heat increases in the melting phase of the material.
In general, the specific heat at constant heat will have values ranging from 1.6 to 2.8 𝐽
𝑔°𝐶, which depends not only on the type of material but also on the state of the material.
A further characteristic of fatty acids is that during the phase change phase, small variations in volume may occur and furthermore, during the phase of discharge and therefore of heat transfer of the fatty acid to the fluid, no phenomenon occurs below cooling, which would make the use of the material very advantageous.
For the carboxylic group, fatty acid based PCMs are chemically and thermally stable, with low corrosion and non-toxic activity.
The raw materials of fatty acids derive from renewable vegetable and animal sources, which would therefore ensure a continuous source of non-polluting supply.
The fatty acid based PCM can be produced by the following procedures:
- Triglycerides present in nature;
- Hydrate of triglyceride acids and their mixtures;
- Esters of fatty acids and triglycerides present in nature;
- Triglyceride products synthesized by hydrogenation and fractionation;
- Synthesized triglyceride products using isomerization and cis-trans fractionation;
- Derived fatty acid derivatives that have the desired temperatures for the freezing point;
- Hydrates of refined fatty acids which have the desired temperatures for the freezing point;
29 - Prepared mixtures essentially produced from any of the previous processing approaches with other chemicals to produce eutectic compositions with the desired temperature range for the freezing point. 
3.3 NON-PARAFFINIC ORGANIC MATERIAL EXAMINATED
As noted in the previous paragraph, non-paraffinic organic materials having good thermodynamic characteristics, they can be used for a wide range of energy production systems such as phase change storage materials.
Having already anticipated that, these materials will be used predominantly for the energy storage of renewable source systems, most of the investment costs will be used for the energy production system therefore trying to save for storage costs.
In addition, that is why the studies focused on low cost materials, for their easy availability, such as organic materials.
In this case, it has been noted that non-paraffinic organic materials have had excellent results and are also preferred to other PCMs because of their low cost.
The study carried out is that of being able to lower costs by trying to exploit waste materials as phase change accumulation materials.
In this case, after having carried out some research, we tried to deepen the study on lard, butter and meat fat produced by a post-cooking process.
These three materials are taken for verifying their feasibility of use in the field of thermal storage and finally comparing them with a generic organic material with phase change as paraffin wax.
Lard is a material used for food obtained through the fusion of elements present in the adipose tissue of the pig. It is commonly used for frying or kneading.
Together with butter, it was decided to use this material for phase-change thermal storage.
Lard consists of 97.28% fat, 0.003% protein, 0.005% water and the remainder of vitamins and minerals.
30 For the energetic characterization of the lard, it has been found very difficult in the research of the thermodynamic properties since the component is almost never used for scientific purposes.
Through research the found thermodynamic properties are density, specific heat (in liquid and solid phase), thermal conductivity and melting temperature.
As far as density is concerned, at 15 °C, it does not have precise values and this is due to the percentage of components and the type of processing.
In fact the value goes from 0.9140 to 0.9430 g/ml and then for the simulation phase a medium value will be used to simplify the data recording process.
The specific heat assumes values equal to 1.3 𝑘𝐽
𝑘𝑔𝐾 in the solid phase and 2.26 𝑘𝐽
𝑘𝑔𝐾 in the liquid phase, values that are appropriate for the study examined.
Through the study carried out by Lentz in 1961 , it is certified that the thermal conductivity of the lard takes a value equal to 0.215 𝑊
𝑚𝐾 at 3 °C while 0.218 𝑊
𝑚𝐾 at -15 °C. This means that, even in this case, the thermal conductivity varies with temperature changes.
In this case, the thermal conductivity is inversely proportional to the temperature and to have values close to the real ones, during the simulation, through these two values we will try to draw a weighting curve.
Finally, the melt temperature instead assumes values of 41 °C, which allows to be able to advance assumptions of feasibility of use of the material for a phase change thermal storage system.
Butter is a derivative of milk and consists mainly of water for 15.11%, of fats for a good 83.59%, of proteins for 1.18% and finally of 0.12% of other waste.
The main composition of the butter is mostly fatty acids and this makes it difficult to calculate its thermodynamic characteristics.
From previous studies, it has been verified that the density of butter, compared to other milk derivatives, is much lower. This is a quantity of raw materials that distinguishes butter from other milk derivatives.
Figure 24 Density of dairy products 
As far as the melting temperature is concerned, the complex composition of the butter, consisting of many fatty acids, makes its calculation difficult.
Common Name Formula Melting Point
Soluble volatile fatty acids
Acetic acid C2H4O2 -16 °C
Propionic acid C3H6O2 -20 °C
Butyric acid C4H8O2 -8 °C
Insoluble volatile fatty acids
Caproic acid C6H12O2 +3 °C
Caprilic acid C8H16O2 +16 °C
Capric acid C10H20O2 +30 °C
Lauric acid C18H36O2 +42 °C
Fixed fatty acids
Myristic acid C14H28O2 +54 °C
Palmitic acid C16H32O2 +62 °C
Stearic acid C18H36O2 +70 °C
Unsaturated fatty acids
Palmitoleic acid C16H30O2 +1 °C
Oleic acid (cis) C18H34O2 +16 °C
Vaccenic acid (trans) C18H34O2 +43 °C Polyunsaturated fatty acids
Linoleic acid C18H32O2 +4 °C
Figure 25 Melting points of single components of dairy products 
32 It is possible to notice, from the previous table in figure 25, the fatty acids that make up milk fat, that is the main component from which butter and other derivatives come from, all have different temperatures.
To simplify the study, on average the butter has a melting temperature that is between 32 and 35 °C until it has completely melted the material at 40 °C.
Figure 26 Melting temperature for some foods 
As for thermal conductivity, its determination remains very complex to solve. As the butter, as well as other organic materials, consisting of many elements, for the calculation of thermal conductivity, and other thermodynamic characteristics, studies have been carried out with the aim of making it easier to calculate.
Figure 27 Thermal properties for each food component 
A very interesting study was made by Brian A. Fricke and Bryan R. Becker , and it was interesting to note that the characteristics of an organic material not only depend on the composition of the element taken into consideration, but also on the temperature.
Obviously every organic material has its own composition and quantity of proteins, fats, fibers and other materials, and therefore for the calculation of the thermal conductivity the formula 𝑘 = ∑ 𝑥𝑖𝑣𝑘𝑖 has been used, where 𝑥𝑖𝑣 corresponds to the volumetric fraction of each individual component of the material and 𝑘𝑖 its thermal conductivity.
Figure 28 Thermal conductivity of dairy products 
34 Through these studies, the interpretation of the calculation of thermal conductivity has led to further theories that made it difficult to calculate and that is why we have tried to simplify the problem by using the result obtained by I.H.Tavman and S. Tavman  where the thermal conductivity assumes a value of 0.227 𝑊
𝑚𝐾 at 15 °C and 0.233 𝑊
𝑚𝐾 at 30 °C.
As can be seen from the table, the thermal conductivity of the butter has a much lower value than the other milk derivatives, which however more or less assumes the same tendency to vary the temperature.
Moreover, thanks to the same study, the value of the density of butter equal to 642.3 𝑘𝑔
𝑚3 is assumed for simplicity.
The same reasoning was made at the specific heat and in this case reference was made to the study carried out by Hammer and Johnson in "The specific heat of milk and milk derivate" , and we have reached the conclusion described in the following table.
Specific heat 𝑱
At 0 °C At 15 °C At 40°C At 60°C
Whey 0.978 0.976 0.974 0.972
Skim Milk 0.940 0.943 0.952 0.963
Whole Milk 0.920 0.938 0.930 0.918
15% Cream 0.750 0.928 0.899 0.900
20% Cream 0.723 0.940 0.880 0.886
30% Cream 0.673 0.983 0.852 0.860
45% Cream 0.606 1.016 0.787 0.793
60% Cream 0.560 1.053 0.721 0.730
Butter 0.512 0.527 0.556 0.580
Butter Fat 0.445 0.467 0.500 0.530
Figure 29 Specific heat of dairy products 
From the table it is observed that the specific heat of the butter takes on low values compared to the other derivatives and therefore the amount of heat that will serve to raise a Kelvin degree one kilogram of butter will be much lower than the amount of heat that is needed for the others derivatives.
35 Furthermore, the growth in the quantity of specific heat is directly proportional to the increase in temperature, which in some dairy products this correlation between specific heat and temperature is not obtainable.
In other cases the specific heat assumes a value of 1.42 𝑘𝐽
𝑘𝑔𝐾 in the solid phase and 2.72 𝑘𝐽
𝑘𝑔𝐾 in the liquid phase.
The butter from a first observation has good thermodynamic performance and therefore has been considered for use as a phase change material for thermal storage systems.
The material not only has excellent thermodynamic characteristics but is easily available, non toxic, does not corrode in contact with other materials and is economical.
Its availability is due to the high use of butter in the food chain, which is why we will investigate the possibility of being able to use waste for a phase change thermal system for space heating or domestic hot water.
3.3.3 MEAT FAT
As third material is taken in consideration, meat fat obtained by a post-cooking process.
This material it is not used as thermal storage process, so it was very difficult research all its thermal characteristics.
First of all, meat fat is principally composed by saturated fat ad by this material are prepared other products, as for example lard.
Its low utilization in thermal field, has made the determination of some thermodynamic characteristics very difficult. In fact, it was possible deriving density, that has a value equal to 930 𝑘𝑔
𝑚3, and thermal conductivity that has a value equal to 0.23 𝑊
While for the specific heat, it was used the same of the lard, for its similar composition.
At the end, also for the melting temperature, no real scientific correspondence has been found, so for simplicity it was adopted the same melting temperature of the lard, 41°C.
For the others thermal elements, not used for our study, is not done a deeper survey.
36 3.3.4 PARAFFINIC WAX
As already mentioned above, unlike the three previous compounds, paraffin wax is one of the most used among phase change organic materials for thermal storage systems.
Being the most exploited, numerous studies have been carried out that have allowed to give a well defined energetic characterization.
In the previous paragraphs it has been shown how the thermodynamic properties of paraffin depends a lot on its chemical composition. In fact, paraffin is an organic component characterized mainly by a long carbon chain. The variation in length of the main chain will affect the properties of the compound.
Figure 30 Variation of thermal properties of paraffinic wax which depends by the number of carbon atoms into the chain 
From the study carried out by Sari, Alkan and Bilgin, it was determined how the temperature and the latent heat not only depends on the length of the chain of carbon atoms but also if we are in the process of melting or solidifying the compound. 
With regard to the specific heat for simplicity, it maintains an almost constant value of 2.13 𝑘𝐽
𝑘𝑔𝐾, during the process it accumulates and independently of the quantity of carbon atoms that make up the material. 
The conductivity of the paraffin wax takes on a value equal to 0.25 𝑊
𝑚𝐾 at a temperature of 25
°C and as you can see, although it is the most used material among those with phase change for the thermal storage systems, the paraffin it has a thermal conductivity very similar to the other two organic materials that will be examined later. 
What will be verified in the next chapter is if the lard and butter can be excellent substitutes as accumulation materials and you can have energy benefits, in addition to the economic ones, to the detriment of the classic paraffin wax.
37 3.4 DSC ANALYSIS
To determine in more detail the energy characterization of the materials that will be taken into consideration, it is considered to undertake the analysis DSC (Differential Scanner Calorimetry).
With the help of the Department of Applied Science and Technology of the Polytechnic of Turin, machinery was used to determine the thermodynamic properties of phase change organic materials.
Differential scanning calorimetry allows direct measurement of the amount of heat emitted or absorbed by the sample through a compensation mechanism, based on maintaining the thermal equilibrium (temperature equality) between sample and reference.
Sample and reference are inserted into two separate cells; their temperature is monitored by means of two thermocouples in contact with the crucibles containing them.
A first electric circuit determines the heating of both cells on the basis of the average measured temperature; this heating is programmed with the temperature growth rate chosen as desired in the interval between 1 and 100 °C per minute.
Figure 31 DSC Analysis machine
Figure 32 Schematic diagram of the measuring cell and of the electric circuits of heating and compensation of the purchased or sold heat of a DSC equipment. On the right, is shown the specimen inserted inside the machine.
A second circuit warms the sample and reference in a differentiated manner, keeping the same at the same temperature even in the presence of exothermic or endothermic phenomena. The amount of energy supplied by the compensation circuit, when these phenomena occur, is equal to the amount of heat involved in the transformation undergone by the sample.
Figure 33 Typical DSC curve 
39 The obtained DSC curve represents the differential heat delivery rate as a function of time or of the average temperature of the system. The maximum sensitivity of the instrument is 0.1 mcal /s.
The speed at which the system compensates for example the heat absorbed during a sample transformation (dH/dt) depends on both the programmed heating rate (dTp/dt) and the thermal resistance R0 according to the equation:
dt dT R dt
dH = • p 0
1 (1) Tp = programmed temperature; R0 = thermal resistance of the system
Therefore, the peaks will grow more or less rapidly depending on these parameters: clearer peaks will be obtained with a higher programmed heating rate and when the gaseous atmosphere in the measuring cell allows faster conduction of heat.
If the heating rate is high, the sample may be in a condition of greater thermodynamic instability, which requires a greater amount of energy consumed in the unit of time to complete the transformation. If the thermal resistance of the system is large, the sample can only acquire energy slowly. Even if the above experimental parameters influence the shape of the peak, the underlying area will be however independent of the experimental conditions adopted, therefore in any case the instrument will provide a correct measurement of the heat involved.
The main limits of the differential scanning calorimetry are in the application temperature range, which extends only between -150 °C and about 700 °C. These limits, in particular with reference to the maximum temperature attainable, are instrumental in nature, and therefore difficult to overcome.
The main limits of the differential scanning calorimetry are in the application temperature range, which extends only between -150 °C and about 700 °C. These limits, in particular with reference to the maximum temperature attainable, are instrumental in nature, and therefore difficult to overcome.
The determination of the onset of a phenomenon consists in the evaluation of the temperature of the system in correspondence of which a deflection of the baseline is observed.